• date post

25-Apr-2022
• Category

## Documents

• view

0

0

Embed Size (px)

### Transcript of 05a - Aggregate Blending - Memphis

Microsoft PowerPoint - 05a - Aggregate BlendingAggregate Blending
Aggregate Blending
To meet the gradation specifications for a concrete or asphalt mix, we usually have to blend aggregate from several sources together. To find an aggregate source with exactly the right gradation is highly improbable.
If we only have to blend two aggregates together, we can usually calculate the proportions directly. If we need to combine three or more aggregates, we have to resort to trial-and-error.
CIVL 3137 2
CIVL 3137 3
blend A B C
i i i i A B Cp f p f p f p
pi x = percent of material x passing sieve i
fx = fraction of blend contributed by material x
Two-Aggregate Example
B
A
50
36
Pick a point in the middle of the gradation band (e.g. 43% passing No. 8 sieve)
CIVL 3137 5
Two-Aggregate Example
No.8 No.8 No.8 blend A A B Bp f p f p 43%
A Bf f 1
No.8 No.8 No.8 blend A A A Bp f p 1 f p 43%
CIVL 3137 6
A44 73f
Af 0.6
Percent Passing
60:40 Blend
Trial-and-Error Solution
Let’s look at the TDOT specification for an asphalt concrete mix that would be used on the shoulders of an interstate highway (411-E).
An asphalt plant in Middle Tennessee had stockpiles of No. 78 stone, natural sand, and screenings. What proportions of these three materials are needed to meet the TDOT specification?
CIVL 3137 10
CIVL 3137 11
.
1½" ¾" 3/8" 4 8 16 30 50 100 200
TDOT 411-E
.
1½" ¾" 3/8" 4 8 16 30 50 100 200
Sand
Aggregate Blending
The TDOT specification requires approximately 13% be retained on the 3/8" sieve but the screenings and sand have nothing retained on that sieve, so all of the coarse sizes will have to come from the crushed stone.
The crushed stone has 38% retained on the 3/8" sieve, so the crushed stone should be roughly 13/38 1/3 of the blend.
CIVL 3137 13
CIVL 3137 14
.
1½" ¾" 3/8" 4 8 16 30 50 100 200
Sand
13% retained
Aggregate Blending
The TDOT specification requires approximately 6% pass the No. 100 sieve but the sand and stone have nothing passing the No. 100 sieve, so all of the fine sizes will have to come from the screenings.
The screenings have 9% passing the No. 100 sieve, so they will have to be 6/9 2/3 of the blend.
This suggests that a blend of 1/3 crushed stone and 2/3 screenings will get us in the ballpark.
CIVL 3137 15
CIVL 3137 16
.
1½" ¾" 3/8" 4 8 16 30 50 100 200
Sand
.
1½" ¾" 3/8" 4 8 16 30 50 100 200
Sand
Aggregate Blending
As we expected, we fit the specifications at the two ends, but we don’t have enough material between the No. 8 and No. 50 sieves. That’s where the sand comes in. Most of its particles are in that size range.
We now need to start adding sand into the blend until we get a gradation curve we’re happy with. As the amount of sand goes up, the amount of screenings and stone will have to go down to make room.
CIVL 3137 18
CIVL 3137 20
.
1½" ¾" 3/8" 4 8 16 30 50 100 200
TDOT 411-E